© 2017, IRJET | Impact Factor value: 5.181 | ISO 9001:2008 Certified Journal | Page 2073
Experimental Investigation of Hybrid Fibre Reinforced Concrete Short
Columns Using Micro Steel Fibre and E-Waste Fibre
Er. Shifina Basheer1
, Er. Minu Antony2
M Tech Student, Dept. of Civil Engineering, Saintgits College of Engineering, Kerala, India2
Assistant Professor, Dept. of Civil Engineering, Saintgits College of Engineering, Kerala, India
This paper present an experimental study on
concrete short columns reinforced with hybrid fiber
under axial loading condition. The strength and
durability of concrete short column improve with the
addition of fiber. Fibers added to the concrete at 0.6, 0.8
and 1% of e-waste and 0.5,1 and 1.5% of micro steel
fiber with respect to the weight of concrete on the
strength criteria of M30. In hybrid fiber concrete, the
micro steel fiber delayed the development of macro
cracks and e-waste fiber helps to improve the
mechanical properties of concrete .When using e-waste
fiber in concrete it reduces the amount of dumping e-
plastic waste into nature. A total of eight column
specimen consisting of one normal RCC column, four
fiber reinforced column and three hybrid fiber reinforced
column were tested. The experimental result reveals that
the optimal percentage addition of fibers to the concrete
was found to be 0.8% of e-waste and 1.5% of micro steel
fiber with respect to the weight of concrete. Result show
that a combination of micro steel and e-waste fibers can
be efficiently used to optimize the behavior of concrete.
Hybrid fiber reinforced short columns were capable of
carrying large amounts of strain than normal RC
Key Words: Hybrid fiber reinforced concrete, short column, Micro steel fiber reinforced concrete (MS-FRC) , E-waste fiber reinforced concrete (EFRC)
In the recent years, the various fibers were developed and used in the construction industries. Steel is mainly used fiber in concrete for various applications. Also glass fiber polythene fibres, carbon fibres, polyamide fibres ,sisal fiber are now developed and also used in construction, industrial and infrastructure development. Some electronic waste fibres can also be used in concrete. Electronic waste is considered more toxic than municipal waste. When e-waste used inconcrete, it reduces the environmental pollution and solid waste problem. E-waste in concrete is the new
revolutionary concept of sustainable concrete. E-waste plastic type fiber of different length, a small size of e-waste plastic will show good result in properties of concrete as compared with the larger size. In this paper, the extracted outer casting of electronic wire was used for making e-waste fiber. Fiber reinforced concrete helps to reduce the crack propagation and increase the mechanical properties compared to the normal concrete. In hybrid concrete, the micro fibers delayed the development of macro cracks and greater strength and crack resistance. It also improve the mechanical properties of concrete. The strength and the corresponding deflection was increase linearly with increasing steel fiber content in concrete. Effect of two or more fibres used in concrete gives the benefits of individual fibres and also improve desired properties of concrete. Hybrid fiber has been shown to be applicable to many types of RC structural elements. Several studies carried out on testing reinforced concrete short columns with different types of fibers. From this studies, we can conclude that to investigate the behavior of hybrid fiber concrete short columns under axial loading condition.
2. LITERATURE REVIEW
© 2017, IRJET | Impact Factor value: 5.181 | ISO 9001:2008 Certified Journal | Page 2074 experimentally investigated the engineering properties of e-
waste concrete and compared with normal specimen. In this paper the Coarse aggregate was partially replaced with HIPS. High impact polystyrene plastic (HIPS) may be used in structural concrete, up to 20% replacement by volume was good and acceptable. Iftekar Gull and M.Balasubramanian (2014) experimentally investigated, the mechanical properties of concrete with different proportions of material. Different proportion of e-waste are used-0%,0.4%,0.6%,0.8%,and 1% with respect to volume of cement. Plastic material is shredded into small pieces of 5cm,4cm and 3cm are used. Small size of e-waste plastic will show good result in properties of concrete as compared with the larger size. Emdad K. Z Balanji ,M Neaz Sheikh and Muhammad N. S Hadi(2016) experimentally investigate behavior HSC with hybrid fiber steel under different loading condition.By the addition of steel fiber in concrete, the strength and ductility of columns improves. The results shows that the specimens reinforced with HSF achieved higher strength and ductility compared to normal concrete. Specimens is tested under different loading conditions. Doo-Yeol Yoo, Hyun-Oh Shin and Young-Soo Yoon (2013)studied on the effect of fiber content on the material and interfacial bond properties of ultra high performance fiber reinforced concrete .Four different volume ratios of micro steel fiber (1%,2%,3%,4%) with respect to volume of concrete are used. 3% steel fiber by volume shows best performance compared to normal concrete.
3. MATERIAL USED
Ordinary Portland cement of Dalmiya brand of grade 53 conforming to IS 12269:1987 was used. The properties of cement are given in the table 1.
Table -1: Properties of Cement
1 Specific gravity 3.15
2 Standard consistency 33% 3 Initial setting time 98 minutes 4 Final setting time 308 minutes
5 Fineness of cement 1.82%
1 Specific gravity 3.15
3.2. Fine Aggregate and Coarse Aggregate
M-sand, free from organic impurities conform to IS 4031: 1988 and crushed stones of 20mm, 12.5mm and 6mm sizes conform to IS 2386: 1963 part 3 were used. Properties of fine and coarse aggregate are shown in Table 2 and gradation curve of fine aggregate are in Figure 2.
Table -2: Properties of Fine and Coarse Aggregate
No Property Result
1 Specific gravity of fine aggregate
2 Specific gravity of coarse aggregate
3 Water absorption 0.51%
0.15 0.3 0.6 1.182.364.75 10
Grading of Fine Aggregate
Figure -2: Gradation curve of fine aggregate
3.3. Super Plasticizer
© 2017, IRJET | Impact Factor value: 5.181 | ISO 9001:2008 Certified Journal | Page 2075
Table- 3: Physical and Chemical Properties of Super
3.4. Micro Steel Fiber
13 mm length size micro steel fiber was used. It helps to increases tensile strength and toughness of concrete.
Table- 4: Properties of Micro Steel Fiber
Fiber Type Brass Coated Straight Steel Type
Dimensions Equivalent diameter 0.2mm and length 13mm
Aspect Ratio 33-35
Tensile Strength 2200-2850 N/mm2
Figure- 3: Micro Steel Fiber
3.5. E-Waste Fiber
Extracted outer casing of electrical wire were used for making e waste fiber in concrete. Diameter of fiber -4mm and length-3 cm size fiber was used. E- plastic waste fiber are shown in figure 4.
Figure- 4: E-Waste fiber
4. EXPERIMENTAL INVESTIGATION
4.1.Concrete Mix Design
Concrete mix design was done as per IS 456:2000 and IS 10262:2009. The mix proportion for M30 mix is given in table 5.
Table -5: Mix Proportion
No. Material Quantity(Kg/m 3)
1 Cement 350
2 Fine Aggregate 760
3 Coarse Aggregate 1220
4 Water 160
5 Super Plasticizer
(0.4%mass of cement) 1.812
6 Water Cement Ratio 0.45
Mix Proportion (C:FA:CA:W) 1:2.17:3.48:0.45
4.2.Design of Column
Design of column was done as per IS 456:2000. As per the
design, 4 numbers of 12mm diameter bars were provided as main reinforcement and 8mm diameter bars are used as transverse reinforcement. The cover provided is 20mm. The reinforcement detail for column is shown in figure 5. Sl. No Property Result
1 Appearance Yellow coloured liquid
2 Ph Minimum 6
3 Volumetric mass at
4 Dosage 0.5-0.3 liter/100kg of
© 2017, IRJET | Impact Factor value: 5.181 | ISO 9001:2008 Certified Journal | Page 2076
Figure -5: Reinforcement details of column
4.2. Test Specimen Details
An experimental research has been planned to study the behavior of short columns having 150 mm×150 mm×700 mm size in-filled with different types of concrete such as normal M30 mix and hybrid fiber reinforced concrete (HFRC). To obtain suitable hybrid fiber reinforced concrete mix for columns several trials was done by standard compression test, flexural test and slit tensile test on cube, beam and cylinder. From the test results the optimum dosages of different fibers was determined. Details of column specimens were given in table 6.
Table- 6: Details of Test Specimen
Specimen Specimen Designation
Percent of Micro Steel
Percent of E- waste
RCC Column C1 0 0
C2 1.5 0
EFRC Column C3 0 0.8
HFRC Column C4 1.5 0.8
4.3. Test setup
Short column were tested on UTM (500kN) as shown in figure 6. The columns were cured for a period of 28 days and then the surface of columns cleaned and white wash were applied for the clear visibility of cracks. The load was applied on the column specimen until the failure took place. The load was applied until the failure took place. Axial strain of column noted at equal interval with help of strain gauge. Then ultimate load and corresponding strain was noted. The ultimate load or fracture load was taken at which the needle of load dial on the UTM returned back. The average of the few trials was taken and the stress-strain graph was plotted.
Figure -6: Test set up
5. RESULTS AND DISCUSSIONS
5.1. Standard Test Results
Compressive strength of concrete cubes for different HFRC mix, MS-FRC mix, EFRC and normal M30 are shown in table 7.
Table- 7: Compressive strength of cubes
mix % of e-waste fibers
% of steel fiber
stress in 28 days(N/mm2)
Mix 0 0 35.76
0 0.5 36.24
MS-FRC 0 1 38.88
0 1.5 39.82
0.6 0 35.05
EFRC 0.8 0 36.24
1 0 34.03
0.8 0.5 36.86
HFRC 0.8 1 39.82
© 2017, IRJET | Impact Factor value: 5.181 | ISO 9001:2008 Certified Journal | Page 2077 From the compression test results of HFRC cubes 1.5%
micro steel fiber and 0.8% e-waste fiber were fixed as the optimum dosage. From the results of compressive strength, split tensile strength and flexural strength of cube, beam and cylinder for normal M30 mix concrete and finalized HFRC mix.
5.2. Short Column Test Result
Axially loaded columns are the one where load acts at the centroid of the column cross-section. The columns were EFRC, MS-FRC,HFRC and is compared with control specimen. Comparison of failure pattern and strain relationships are presented. The ultimate load carrying capacities are calculated and are plotted. Hybrid fiber reinforced column specimen shows increase in ultimate load carrying capacity compared to normal specimen. In micro steel fiber reinforced column 75.08% increase in ultimate load carrying capacity. Increase in load carrying capacity is due to the effect of fibers, they provide structural integrity to concrete and prevent the formation of micro cracks confinement effect provided by steel tube The ultimate load carrying capacities of each column specimens are graphically plotted and compared with the control specimens.
0 100 200 300 400 500 600
control specimens micro steel fiber
e-waste fiber Hybrid fiber
Figure -7 : ultimate load values
Test was continued until the failure of specimen took place. When the short columns are axially loaded, the reinforcement steel and concrete experience stress. Found that HFRC short column showed higher resistance compared
with normal RC column. Failure mode of specimen divided into three types based on their material properties and geometric configuration. From the failure patterns of the normal RC specimens it is clear that the failure occurs mainly due to crushing. As long as it is a short column there is no chance of buckling. Due to crushing failure the cracks are mainly seen at the top and bottom of the column specimen. The ultimate load carrying capacities of each column specimens are graphically plotted and compared with the control specimens.
In order to study the behavior of concrete columns, to plot appropriate analytic strain graph. The better stress-strain graph results in reliable estimation of strength and deformation behavior of the structural members. The stress strain curve for normal specimen, EFRC, MS-FRC and hybrid fiber reinforced concrete short column were obtained. Figure 8 shows the stress strain curve for hybrid fiber reinforced concrete short column. Figure 8 shows the stress strain curve of normal specimen.
0 5 10 15 20
© 2017, IRJET | Impact Factor value: 5.181 | ISO 9001:2008 Certified Journal | Page 2078
0 5 10 15 20
0.002 0.004 0.006 0.008 0.01
Concrete short columns with or without fiber content were tested under axial loading condition. The behavior of short columns was analyzed with respect to ultimate load carrying capacity, and failure modes. From the experimental study the following conclusions were drawn.
Hybrid fiber reinforced columns have 81%increases in maximum load carrying capacity than that of the normal RC column.
In micro steel fiber reinforced column 75.08% increase in ultimate load carrying capacity. Increase in load carrying capacity is due to the effect of fibers, they provide structural integrity to concrete and prevent the formation of micro cracks confinement effect provided by steel tube.
In e-waste fibre reinforced concrete columns have 20.24 % increase in load compared to normal column. Hybrid fiber reinforced concrete short columns were
capable of carrying large amounts of strain than normal RC column.
 Arjun Ramakrishna Kurup and K. Senthil Kumar (2016)”Novel fibrous concrete mixture made from recycled PVC fibers from electronic waste” J. Hazard.Toxic Waste ASCE.
 Ashwini Manjunath B(2016)” Partial replacement of E-plastic waste as coarse aggregate in concrete” Environmental science, ELSEVIER
 K.Senthil Kumar and K.Baskar(2015)”Development of Eco-friendly concrete incorporating recycled high-impact polystyrene from hazardous Electronic waste. J. Hazard.Toxic Waste .
 Iftekar Gull and M.Balasubramanian(2014)” A new paradigm on experimental investigation of concrete for e- plastic waste management” J.Eng Trend and Tech
 Emdad K. Z Balanji ,M Neaz Sheikh and Muhammad N. S Hadi(2016)”Performance of high strength concrete columns reinforced with hybrid steel fiber under different loading conditions
 Doo-Yeol Yoo,Hyun-Oh Shin and Young-Soo Yoon (2013)”Material and bond properties of ultra high performance fiber reinforced concrete with micro steel fiber”. J.Composites, ELSEVIER.
Selina Ruby G., Geethanjali C., Jaison Varghese, P. MuthuPriya(2014)”Influence Of Hybrid Fiber On Reinforced Concrete ‘International Journal Of Advanced Structures And Geotechnical Engineering, Vol. 03.
 Yin Chi, A.M.ASCE; LihuaXu; and Yuanyuan Zhang ‘Experimental Study on Hybrid Fiber–Reinforced Concrete Subjected to Uniaxial Compression’ American Society of Civil Engineers (2014).
Figure- 9: Stress train behavior of HFRC short column